Electrocomponent Science and Technology, 1981, Vol. 8, pp. 151-157
(C) 1981 Gordon and Breach Science Publishers, Inc.
Printed in Great Britain
FUNDAMENTAL CHARACTERISTICS OF
SOLVENT-SOLUBLE POLYIMIDE RESIN AS A POLYMER
FOR HYBRID APPLICATIONS
Department of Electrical Engineering, Faculty of Technology, Tokyo Metropolitan University, Tokyo,
Reliability Section, Electronic Device Division, Electrotechnical Laboratory, Ibaraki Prefecture, Japan
Japan Technological Research and Development Laboratories, Co., Kokubunji-shi, Tokyo, Japan
Polyimide resin of solvent-soluble type, which is called "X-resin" in short, was discovered lately. It is soluble in
dimethylacetoamid (DMAc), and new extensive applications are expected.
Some physical, chemical and electrical characteristics are studied from the viewpoint of polymer material for hybrid
application. Particularly comparison of the characteristics of X-resin specimens before and after long term exposure
to humid and hot environments were made, remembering that electronic devices often operate under such conditions
From the results obtained up to now, no conspicuous difference seems to exist between the characteristics of X-resin
and those of the conventional (i.e., solvent-insoluble) resins, as published in various literature. It should be noted,
however, that some unusual effects, i.e., the remarkable increase in surface resistivity a, the evident decrease in tan 6,
etc., were found in X-resin specimens after going through the above-mentioned damp-hot test. All those effects are
contrary to the usual concepts of deterioration of polymer materials, but are rather advantageous for hybrid
application. It is also worth noticing that silver migration into X-resin seems scarcely to occur.
Furthermore, new prospective uses of X-resin for printed wiring boards, packaging materials, binder for paste
materials, etc., are investigated.
Polyimide resins have outstanding physical, chemical
and electrical characteristics combined with high
thermal stability over a wide temperature range.
Nevertheless their applications have been restricted to
some particular uses in extreme environments, and they
have scarcely been applied to hybrid or
microelectronics devices. Manufacturers will encounter
two serious problems when they attempt to use
polyimide resin. One is the extreme expensiveness and
the other is the awkwardness of forming and
processing, since polyimides have been considered
neither to melt nor to have any organic solvent.
However, the former may be tolerated if the latter is
solved, and extensive uses are developed. In
consequence, the demands for polyimide resins rise
A new type of polyimide resin, which was called
"X-resin" in short, found very recently. A remarkable
feature of X-resin is that it has "specific"
solvent-solubility similar to such usual linear polymers
as polystyrene, etc., i.e., it can dissolve in a specific
organic solvent even if it is once cured. Since it can be
formed or processed far more easily than conventional
polyimides, various new and extensive applications are
looked forward to unless it has any fatal disadvantage
in its properties.
Thus the physical, chemical and electrical
characteristics of X-resin began to be studied as a
possible polymer material for hybrid application. First
of all, various characteristics of X-resin are compared
152 E. WATANABE, K. KANOU AND T. KUBOTA
with those of conventional polyimides. Damp-heat tests
are also achieved for film specimens of X-resin,
considering that in Japan electronic devices are often
operated under humid conditions. In fact, moisture is
the cause of some kinds oftroubles in various electronic
devices. Among these, a typical and serious one is
metal migration into polymer materials.
From the results obtained by means of infra-red
spectra studies, no conspicuous difference has been
found between chemical structures of X-resin and
conventional polyimide resin.
3. SPECIMENS AND CONDITIONS FOR
2. CHEMISTRY OF X-RESIN
Conventional polyimides are formed typically by three
stages as shown in Figure 1. Chemical reactions of
X-resin formation are considered to be substantially
similar to those in Figure 1, except for a few modi-
fications of conditions. Forming and processing of con-
ventional polyimide resins are usually made for solvent-
soluble intermediate products at stage (II) (polyamic
acid), because the final product at stage (III) (i.e.,
polyimide resin) has no solvent-solubility. On the
other hand, X-resin dissolves in a specific solvent.
dimethylacetamide (DMAc), though it is considered to
be equivalent to a final product at stage (III).
P,yrome t c
(25C to 50C)
4,4 Diamino phenyl ether
in a solvent such as
dimeth acetami de(DMAc
(IO0C to 300C) Catalyst(metalc
FIGURE Chemical reactions of polyimide formation.
X-resin specimens for various evaluation tests are
prepared as follows: X-resin powder dissolves in
DMAc at a ratio of approximately 1 vs. 10 in weight to
become a paste-like disposition. Then it is formed in
sheets or films on a suitable flat plate. They are cured at
100C for 30 minutes, and further heat-treated at
200C for one hour for the purpose of sufficient
volatilization of solvent. In addition, a sample
heat-treated at 300C is added for thermal analysis.
Thickness of the specimens is between 100 and 200 #m.
Temperature and relative humidity for damp heat
tests are usually determined respectively at 40 +_ 2C
and 90-95% according to JIS (Japan Industrial
Standards) C5023 "Damp Heat (Steady State) Testing
Method for Electronic Components". The term of
exposure can be selected from five steps between 48
and 1,000 hours. As for temperature, however, a
somewhat severer condition, i.e., 70C, has been
employed in this study, in order to facilitate the
environmental deterioration of polymer specimens.
4. TEST RESULTS AND EVALUATIONS
TGA and DTA Thermogravimetric analysis (TGA)
and differential thermal analysis (DTA) are achieved
for three kinds of X-resin samples, and also for two
kinds of conventional polyimide on the market for the
purpose of comparative evaluation of the thermal
resistance of X-resin. The specifications of those five
Specifications of polyimide samples for thermal analysis.
Sample Trade name Condition
A heat-treated at 200C
B X-resin heat-treated at 300C
C powder sample (before cured)
D Kaptnb heat-treated at 300CE Torayneece
aTentative name: Japan Technological Research &
Development Laboratories, Ltd.
CToray Industries, Inc.
SOLVENT-SOLUBLE POLYIMIDE RESIN FOR WIRING BOARDS 153
kinds of samples (sample A-E) are put together in
Table I. The resultant TGA and DTA curves for
X-resins are shown in Figure 2, and those for
conventional polyimides are shown in Figure 3. From
TGA curves in Figure 2, it is observed that for sample
A and B the first apparent decreases in weight begin
from the temperatures a little over 200 and 300C
respectively. Note that those temperatures roughly
coincide with those of heat treatments for each sample
(cf. Table I). Moreover, from DTA curves in Figure 2,
it is found that the above-mentioned decreases in
weight are accompanied with endothermic chemical
processes. The slight decrease in weight is also
observed in sample C at a temperature as low as less
than 100C, and is surely due to the desorption of gases
absorbed on the surfaces of powder particles of X-resin
sample. As for the conventional polyimide sample D
and E, neither a decrease in weight nor a chemical
reaction is observed up to as high as near 500C, as
shown on TGA and DTA curves in Figure 3. Thus the
first decreases in weight of samples A and B should
be caused by volatilization of residual solvent.
It is obvious that for all X-resin samples (A-C) the
second abrupt decreases in weight begin from the
coincident temperature, i.e., about 450C, as shown in
TGA curves in Figure 2. Those second decreases are all
accompanied with somewhat complicated exothermic
and/or endothermic reactions, as also shown in DTA
curves in Figure 2. Thus those reactions are considered
to correspond to thermal crackings of X-resin.
In consequence the thermal resistance of X-resin is a
little lower than that of conventional polyimides, but it
can be improved remarkably by means of heat
treatment at a relatively high temperature so that the
residual solvent volatilizes completely.
Electrical Characteristics DC and AC measurements
were made to obtain fundamental electrical
characteristics of X-resin. The resultant values for
sample A are shown in Table II, together with those of
conventional polyimides and, for ready comparison,
some other resins which are often used in hybrid
devices. Note that frequencies for AC measurements
are different among various specimens.
The insulation resistance of X-resin has no
substantial difference from conventional polyimides,
and is roughly equal to or rather higher than those of
epoxy resins. Taking the difference in measuring
frequency into consideration, tan 6 of X-resin does not
seem to be so large.
0 I00 200 300 400 500 600
FIGURE 2 Results of TGA and DTA for X-resin samples.